Flax has a long and fascinating history. This plant was domesticated around 8,000 bce1 in the Fertile Crescent area2, first for its seeds and then for its fibres1,3. Although its uses existed long before domestication, residues of flax yarn dated 30,000 years ago have been found in the Caucasus area4. However, Ancient Egypt laid the foundations for the cultivation of flax as a textile fibre crop5. Today flax fibres are used in high-value textiles and in natural actuators6 or reinforcements in composite materials7. Flax is therefore a bridge between ages and civilizations. For several decades, the development of non- or micro-destructive analysis techniques has led to numerous works on the conservation of ancient textiles. Non-destructive methods, such as optical microscopy8 or vibrational techniques9,10, have been largely used to investigate archaeological textiles, principally to evaluate their degradation mechanisms and state of conservation. Vibrational spectroscopy studies can now benefit from synchrotron radiation11 and X-ray diffraction measurement in the archaeometric study of historical textiles12,13. Conservation of mechanical performance and the ultrastructural differences between ancient and modern flax varieties have not been examined thus far. Here we examine the morphological, ultrastructural and mechanical characteristics of a yarn from an Egyptian mortuary linen dating from the early Middle Kingdom (Eleventh Dynasty, ca. 2033–1963 bce) and compare them with a modern flax yarn to assess the quality and durability of ancient flax fibres and relate these to their processing methods. Advanced microscopy techniques, such as nano-tomography, multiphoton excitation microscopy and atomic force microscopy were used. Our findings reveal the cultural know-how of this ancient civilization in producing high-fineness fibres, as well as the exceptional durability of flax, which is sometimes questioned, demonstrating their potential as reinforcements in high-technology composites.
This is a preview of subscription content
Subscribe to Journal
Get full journal access for 1 year
only $9.92 per issue
All prices are NET prices.
VAT will be added later in the checkout.
Tax calculation will be finalised during checkout.
Rent or Buy article
Get time limited or full article access on ReadCube.
All prices are NET prices.
The open-source and commercial software used for data analysis are referenced in the Methods section.
van Zeist, W. & Bakker-Heeres, J. A. H. Evidence for linseed cultivation before 6000 bc. J. Archaeol. Sci. 2, 215–219 (1975).
Hopf, M. in The Domestication and Exploitation of Plants and Animals (ed. Dimbleby, G.) Pt. III, Ch. 6 (2008).
Herbig, C. & Maier, U. Flax for oil or fibre? Morphometric analysis of flax seeds and new aspects of flax cultivation in late Neolithic wetland settlements in southwest Germany. Veg. Hist. Archaeobot. 20, 527 (2011).
Kvavadze, E. et al. 30,000-year-old wild flax fibers. Science 325, 1359 (2009).
Heer, O. Prehistoric culture of flax. Nature 7, 453 (1873).
le Duigou, A. & Castro, M. Evaluation of force generation mechanisms in natural, passive hydraulic actuators. Sci. Rep. 6, 18105 (2016).
Mohanty, A. K., Vivekanandhan, S., Pin, J.-M. & Misra, M. Composites from renewable and sustainable resources: challenges and innovations. Science 362, 536–542 (2018).
Bruni, S. et al. Analysis of an archaeological linen cloth: the shroud of Arquata. Radiat. Phys. Chem. 167, 108248 (2020).
Edwards, H. G. M., Ellis, E., Farwell, D. W. & Janaway, R. C. Preliminary study of the application of Fourier Transform Raman Spectroscopy to the analysis of degraded archaeological linen textiles. J. Raman Spectrosc. 27, 663–669 (1996).
Kavkler, K., Gunde-Cimerman, N., Zalar, P. & Demšar, A. FTIR spectroscopy of biodegraded historical textiles. Polym. Degrad. Stab. 96, 574–580 (2011).
Kavkler, K., Šmit, Ž., Jezeršek, D., Eichert, D. & Demšar, A. Investigation of biodeteriorated historical textiles by conventional and synchrotron radiation FTIR spectroscopy. Polym. Degrad. Stab. 96, 1081–1086 (2011).
Müller, M. et al. Identification of ancient textile fibres from Khirbet Qumran caves using synchrotron radiation microbeam diffraction. Spectrochim. Acta Part B At. Spectrosc. 59, 1669–1674 (2004).
Herrera, L. K. et al. Identification of cellulose fibres belonging to Spanish cultural heritage using synchrotron high resolution X-ray diffraction. Appl. Phys. A 99, 391–398 (2010).
Weiss, E. & Zohary, D. The Neolithic southwest Asian founder crops: their biology and archaeobotany. Curr. Anthropol. 52, S237–S254 (2011).
Botany of flax. Nature 170, 557–559 (1952).
Sertse, D., You, F. M., Ravichandran, S. & Cloutier, S. The genetic structure of flax illustrates environmental and anthropogenic selections that gave rise to its eco-geographical adaptation. Mol. Phylogenet. Evol. 137, 22–32 (2019).
Braun, A. Plants of ancient Egypt. Sci. Am. 173, 2760 (1879).
Diederichsen, A. & Hammer, K. Variation of cultivated flax (Linum usitatissimum L. subsp. usitatissimum) and its wild progenitor pale flax (subsp. angustifolium (Huds.) Thell.). Genet. Resour. Crop Evol. 42, 263–272 (1995).
Kawami, T. S. A craft in antiquity. Science 256, 1065–1066 (1992).
André, J. in Pline l’Ancien, Histoire naturelle (ed. Budé, G.) 549–550 (1964).
Goudenhooft, C., Bourmaud, A. & Baley, C. Varietal selection of flax over time: evolution of plant architecture related to influence on the mechanical properties of fibers. Ind. Crops Prod. 97, 56–64 (2017).
Baley, C. & Bourmaud, A. Average tensile properties of French elementary flax fibers. Mater. Lett. 122, 159–161 (2014).
Chemikosova, S. B., Pavlencheva, N. V., Gur’yanov, O. P. & Gorshkova, T. A. The effect of soil drought on the phloem fiber development in long-fiber flax. Russ. J. Plant Physiol. 53, 656–662 (2006).
Bourmaud, A., Gibaud, M., Lefeuvre, A., Morvan, C. & Baley, C. Influence of the morphology characters of the stem on the lodging resistance of Marylin flax. Ind. Crops Prod. 66, 27–37 (2015).
Bourmaud, A., Beaugrand, J., Shah, D., Placet, V. & Baley, C. Towards the design of high-performance plant fibre composites. Prog. Mater. Sci. 97, 347–408 (2018).
Goudenhooft, C., Bourmaud, A. & Baley, C. Study of plant gravitropic response: exploring the influence of lodging and recovery on the mechanical performances of flax fibers. Ind. Crops Prod. 128, 235–238 (2019).
Hernandez-Estrada, A., Gusovius, H.-J., Müssig, J. & Hughes, M. Assessing the susceptibility of hemp fibre to the formation of dislocations during processing. Ind. Crops Prod. 85, 382–388 (2016).
Hughes, M. Defects in natural fibres: their origin, characteristics and implications for natural fibre-reinforced composites. J. Mater. Sci. 47, 599–609 (2012).
Le Duc, A., Vergnes, B. & Budtova, T. Polypropylene/natural fibres composites: analysis of fibre dimensions after compounding and observations of fibre rupture by rheo-optics. Compos. Part A Appl. Sci. Manuf. 42, 1727–1737 (2011).
Foulk, J., Akin, D. & Dodd, R. Influence of pectinolytic enzymes on retting effectiveness and resultant fiber properties. BioResources 3, 155–169 (2008).
Eder, M., Arnould, O., Dunlop, J. W. C., Hornatowska, J. & Salmen, L. Experimental micromechanical characterisation of wood cell walls. Wood Sci. Technol. 47, 163–182 (2012).
Jäger, A., Bader, T., Hofstetter, K. & Eberhardsteiner, J. The relation between indentation modulus, microfibril angle, and elastic properties of wood cell walls. Compos. Part A Appl. Sci. Manuf. 42, 677–685 (2011).
Capron, M. et al. Mechanical characterization of developing tension wood fibre wall by atomic force microscopy. In 8th Plant Biomechanics International Conference 224–225 (Nagoya, 2015).
Bader, T. K., de Borst, K., Fackler, K., Ters, T. & Braovac, S. A nano to macroscale study on structure–mechanics relationships of archaeological oak. J. Cult. Herit. 14, 377–388 (2013).
Shaw, C. Cone Beam Computed Tomography (Taylor & Francis, 2014).
V.P. and G.H. sincerely thank P. Malécot and the MIFHySTO research platform (FEMTO-ST, UTINAM and ICB institutes) at Université Bourgogne Franche-Comté (UBFC) for the technical and scientific support provided for nano-tomography experiments; X. Falourd and L. Foucat (INRAE, BIBS platform) for NMR investigations. We thank the INTERREG IV Cross Channel programme for funding this work through the FLOWER project (grant no. 23); SOLEIL Synchrotron for funding the 99180266 and 99200015 in-house proposals; and the EIPHI Graduate school (contract “ANR-17-EURE-0002”).
The authors declare no competing interests.
Peer review information Nature Plants thanks the anonymous reviewers for their contribution to the peer review of this work.
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Photos from permanent collections of Le Louvre and the British Museum or from non-exhibited collections of Le Louvre Museum.
SEM images, tomography images and distribution of diameters.
SEM images and SHG images.
Source data of distribution of indentation modulus, indentation modulus profiles and processed AFM images.
About this article
Cite this article
Melelli, A., Shah, D.U., Hapsari, G. et al. Lessons on textile history and fibre durability from a 4,000-year-old Egyptian flax yarn. Nat. Plants 7, 1200–1206 (2021). https://doi.org/10.1038/s41477-021-00998-8